Download presentation

Presentation is loading. Please wait.

Published byValerie Trepp Modified over 2 years ago

1
Connie B. Roth, Chris A. Murray and John R. Dutcher Department of Physics University of Guelph Guelph, Ontario, Canada N1G 2W1 COMPLEX FLOW OF NANOCONFINED POLYMERS

2
instabilities in freely-standing liquid films hole growth in freely-standing PS films – ideal geometry for probing complex flow – shear thinning – convective constraint release relaxation mechanism – hole growth occurs for T comparable to T g bulk hole growth in freely-standing PS/PI/PS trilayer films – holes in central PI layer summary & conclusions OUTLINE

3
CURRENT PROJECTS POLYMERS BIOPOLYMERS BACTERIAL CELLS molecular mobility – glass transition & hole growth instabilities & pattern formation biodegradable polymers polypeptides & proteins – lipid membranes & polymer brushes bacterial adhesion & physical properties of bacteria & biofilms

4
to measure structure, dynamics, interaction forces, molecular conformations, adsorption kinetics, we use – atomic force microscopy – ellipsometry – surface plasmon resonance – quartz crystal microbalance – optical tweezers – TIRF – infrared techniques (PM-IRRAS, ATR-FTIR) – surface circular dichroism – TEM – differential pressure techniques SURFACE-SENSITIVE PROBES

5
THIN LIQUID FILMS thin liquid films occur in everyday life – adhesives (superglue) – lubricants (on cornea of eye, engine piston) – spray coatings (paint, herbicides, fibers) – printing (ink on transparency or tape) – soap bubbles & films – foams (shaving cream, cappuccino) – water films (water spotting, hydroplaning) stability desirable/ essential stability undesirable

6
hole radius grows linearly with time [Taylor, Proc. Roy. Soc. (1959)] [Culick, J. Appl. Phys. (1960)] t – fluid collects in a rim – rest of film undisturbed R t HOLE GROWTH IN NON-VISCOUS FILMS

7
h POLYMER MOLECULES polymers are complex molecules – different length scales ranging from segment size to overall chain size R EE ~ M w 0.5 – different time scales ranging from segmental relaxation to diffusion of entire molecules R EE – effect of confinement in thin films – changes in conformation & dynamics

8
hole radius grows exponentially with time [Debrégeas et al., PRL (1995)] t – no rim – film thickens uniformly HOLE GROWTH IN VISCOUS FILMS

9
FREELY-STANDING FILM PREPARATION spincoat polymer solution onto mica substrate anneal film under vacuum transfer film onto water surface capture film on holder containing 4 mm diameter hole high molecular weight, monodisperse polymers dissolved in good solvents

10
– plug flow – driven by surface tension – polymer chains become aligned near edge of hole HOLE GROWTH IN POLYMER FILMS 10 m at edge of hole; into rest of film

11
optical microscopy of freely- standing polystyrene films –M w = 717k –96 nm < h < 372 nm –T = 115 o C (T g bulk = 97 o C) –exponential hole growth –decrease in viscosity for increasing strain rate –consistent with shear thinning [Dalnoki-Veress et al., PRE 59, 2153 (1999)] PREVIOUS HOLE GROWTH IN PS FILMS

12
SHEAR THINNING OF POLYMERS decrease in viscosity with increasing shear strain rate – shear thinning only observed for entangled polymers [Peterlin, Adv. Macromol. Chem. 1, 225 (1968)] – is M w -independent in nonlinear regime [Stratton, J. Colloid Interf. Sci. 22, 517 (1966)] log 00 log PS of diff M w

13
SHEAR THINNING IN FREELY-STANDING PS FILMS use growth time to obtain viscosity at edge of hole plot / 0 versus reduced shear strain rate results consistent with viscous flow in presence of shear thinning different T, M w and h optical microscopy + differential pressure experiment [Roth & Dutcher, PRE 72, 021803 (2005)]

14
FLOW AT SUCH LOW TEMPERATURES? in bulk, viscosity 0 ~ 10 12 Pas at T ~ T g – expect both viscous and elastic effects important – late stage hole growth is well-described by viscous flow previous studies of crazing of PS films [Berger & Kramer, Macro (1987)] – chain scission at low temperatures – chain disentanglement at strain rates & higher temps – for M w = 1800k: T > 70 o C for ˙ = 4.1 x 10 -6 s -1 T > 90 o C for ˙ ~ 10 -2 s -1 comparable strain rates & temps for hole growth 1.5 x 10 -4 s -1 < ˙ < 2 x 10 -2 s -1 for 101 o C < T < 117 o C

15
TRANSITION IN HOLE GROWTH measure R(t) for single hole using optical microscopy – linear growth at early times – velocity v – exponential growth at late times – growth time – range of times for linear growth decreases with – increasing T – decreasing M w R = R o + v t R = R o exp(t / ) PS M w = 2240k, h = 79 nm at T = 103 o C [Roth et al., PRE 72, 021802 (2005)]

16
TRANSIENT BEHAVIOR scale axes: ln[R(t)/R( )] vs t/ – data sets coincide for t > isolate transient – single exponential decay time 1 M w = 717k h = 125 nm

17
TRANSITION IN HOLE GROWTH measure R(t) for single hole using optical microscopy – linear growth at early times – velocity v – exponential growth at late times – growth time – range of times for linear growth decreases with – increasing T – decreasing M w R = R o + v t R = R o exp(t / ) PS M w = 2240k, h = 79 nm at T = 103 o C [Roth et al., PRE 72, 021802 (2005)]

18
TRANSIENT BEHAVIOR scale axes: ln[R(t)/R( )] vs t/ – data sets coincide for t > isolate transient – single exponential decay time 1 refer t to t 0 for which R(t 0 ) = 0 – overlap of data – decay time 1 scales with M w = 717k h = 125 nm

19
FITTING FUNCTION FOR R(t) empirically, R(t) data for all times well fit by – equivalent to time-dependent viscosity (t) – described by a three-component spring & dashpot model where is viscosity for t >> 1 single relaxation time E

20
FITS TO R(t) DATA 3 fitting parameters: R 0 value at start of measurements (t = 0) exponential hole growth time 1 longest relaxation time M w = 717 × 10 3 h = 90 nm

21
RELATIONSHIP BETWEEN AND 1 and 1 have similar temperature dependence with 1 ~ /2 data 1 data / 1 = 2.2 ± 1.4]

22
TUBE MODEL FOR POLYMER DYNAMICS low shear rate ˙ < d -1 reptation + contour length fluctuations (CLF) intermediate shear rate d -1 < ˙ < R -1 convective constraint release (CCR) high shear rate R -1 < ˙ chain stretch [Graham, Likhtman, McLeish, and Milner, J. Rheol (2003)] d Reptation time R Rouse time Hole growth at T = 101 o C d -1 ~ 10 -6 - 10 -10 s -1 R -1 ~ 10 -4 - 10 -7 s -1 ˙ ~ 10 -4 s -1 hole growth at lowest temperatures occurs in the intermediate to high shear rate regimes – relaxation via CCR (no rotation in flow) – since ˙ = 2 / expect 1 ~ ˙ -1 ~ / 2 → data consistent with CCR

23
DIFFERENTIAL PRESSURE EXPERIMENT differential pressure experiment [Roth et al., RSI 74, 2796 (2003); Roth & Dutcher, PRE 72, 021803 (2005)] – maintain pressure difference across PS film – track piston position as a function of time PS, M w = 2240k, h = 69 nm, T = 98 o C

24
DPE RESULTS FOR FREELY-STANDING PS FILMS temperature dependence of hole growth time – M w = 717k, 2240k – 51 nm < h < 98 nm – 92 o C < T < 105 o C – consistent with shear thinning – despite large differences in T g, onset temperature for hole formation is comparable to T g bulk for all films [Roth et al., RSI 74, 2796 (2003); Roth & Dutcher, PRE 72, 021803 (2005)]

25
FREELY-STANDING TRILAYER FILMS trilayer films with central fluid layer and solid capping layers – periodic lateral morphology forms upon heating due to amplification of thermal fluctuations PS/PI/PS [K. Dalnoki-Veress et al., PRL 82, 1486 (1999)] [C.A. Murray et al., PRE 69, 061612 (2004)]

26
HOLE GROWTH IN PS/PI/PS TRILAYERS hole growth in PS freely-standing films – uniform thickening of films – absence of rim at edge of hole hole growth in PS/PI/PS freely-standing films – holes form & grow in central PI layer – distinct rim at edge of hole

27
HOLE GROWTH IN PS/PI/PS TRILAYERS presence of rim verified using atomic force microscopy (AFM) optical microscopy AFM [C.A. Murray et al. (2006)] h = 50 nm, L = 75 nm

28
HOLE GROWTH IN PS/PI/PS TRILAYERS radius of hole in PI layer measured at fixed temperature T = 110 o C fix PS thickness L vary PI thickness h fix PI thickness h vary PS thickness L [C.A. Murray et al. (2006)]

29
HOLE GROWTH IN PS/PI/PS TRILAYERS relevant factors that determine hole growth in PI layer – surface & PS/PI interfacial energies – bending energy of PS layers – dispersion interaction between the PS/air interfaces – can understand slowing of hole growth with increase in h & L

30
SUMMARY hole growth in freely-standing PS films – two different experiments – shear thinning – convective constraint release – hole growth occurs at temperatures comparable to T g bulk hole growth in fs PS/PI/PS films – qualitatively different hole growth – hole growth in PI determined by PS

Similar presentations

Presentation is loading. Please wait....

OK

SNPIT & RC,UMRAKH.

SNPIT & RC,UMRAKH.

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on understanding marketing management Ppt on network theory Free ppt on mobile number portability vodafone Respect for kids ppt on batteries Ppt on two point perspective lesson Ppt on pre ignition Ppt on wildlife and vegetation conservation Ppt on solar power projects Ppt on job evaluation examples Ppt on tribal group of india